#------------------------------------------------------------------------------
#$Date: 2016-03-23 02:32:24 +0100 (Wed 23 de Mar de 2016) $
#$Revision: 179250 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/70/4317030.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4317030
loop_
_publ_author_name
'Geng Bang Jin'
'Emilie Ringe'
'Gary J. Long'
'Fernande Grandjean'
'Moulay T. Sougrati'
'Eun Sang Choi'
'Daniel M. Wells'
'Mahalingam Balasubramanian'
'James A. Ibers'
_publ_section_title
;
 Structural, Electronic, and Magnetic Properties of UFeS3 and UFeSe3
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              10455
_journal_page_last               10467
_journal_paper_doi               10.1021/ic101474e
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'U Fe S3'
_chemical_formula_sum            'Fe S3 U'
_chemical_formula_weight         390.06
_chemical_name_common            'Uranium iron sulfide'
_chemical_name_systematic
; 

 ? 

;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   3.80090(10)
_cell_length_b                   11.6148(4)
_cell_length_c                   8.7022(3)
_cell_measurement_reflns_used    1979
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.42
_cell_measurement_theta_min      2.92
_cell_volume                     384.17(2)
_computing_cell_refinement       'APEX2 v2.0-2 (Bruker, 2005)'
_computing_data_collection       'APEX2 v2.1-4 (Bruker, 2007)'
_computing_data_reduction        'SAINT version 7.23a (Bruker, 2005)'
_computing_molecular_graphics    'CrystalMaker for Windows ver. 2.0.6 (2008)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.966
_diffrn_measured_fraction_theta_max 0.966
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0102
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2198
_diffrn_reflns_theta_full        28.45
_diffrn_reflns_theta_max         28.45
_diffrn_reflns_theta_min         3.51
_exptl_absorpt_coefficient_mu    47.256
_exptl_absorpt_correction_T_max  0.2805
_exptl_absorpt_correction_T_min  0.0385
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'faces indexed'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.744
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             664
_exptl_crystal_size_max          0.354
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.031
_refine_diff_density_max         1.511
_refine_diff_density_min         -1.539
_refine_diff_density_rms         0.357
_refine_ls_extinction_coef       0.0074(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.417
_refine_ls_matrix_type           full
_refine_ls_number_parameters     20
_refine_ls_number_reflns         285
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.417
_refine_ls_R_factor_all          0.0149
_refine_ls_R_factor_gt           0.0149
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc 

 [1.00000+0.00000exp(0.00(sinθ/λ)²)]/ 

   [σ²(Fo²)+0.0000+0.0000*P+(0.0269P)²+0.0000sinθ/λ] 

 where P = 1.00000Fo² + 0.00000Fc² 

;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0430
_refine_ls_wR_factor_ref         0.0430
_reflns_number_gt                285
_reflns_number_total             285
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic101474e_si_002_4.cif
_cod_data_source_block           UFeS3296K
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4317030
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
U U 0.0000 0.755401(17) 0.2500 0.00966(18) Uani 1 4 d S . .
Fe Fe 0.0000 0.0000 0.0000 0.0145(3) Uani 1 4 d S . .
S1 S 0.0000 0.35825(9) 0.05728(11) 0.0095(3) Uani 1 2 d S . .
S2 S 0.0000 0.08297(13) 0.2500 0.0103(3) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
S2 U S2 87.00(4) 5_455 5 ?
S2 U S1 140.91(2) 5_455 14_556 ?
S2 U S1 80.93(2) 5 14_556 ?
S2 U S1 80.93(2) 5_455 5_455 ?
S2 U S1 140.91(2) 5 5_455 ?
S1 U S1 129.53(4) 14_556 5_455 ?
S2 U S1 140.91(2) 5_455 5 ?
S2 U S1 80.93(2) 5 5 ?
S1 U S1 73.53(3) 14_556 5 ?
S1 U S1 85.41(3) 5_455 5 ?
S2 U S1 80.93(2) 5_455 14_456 ?
S2 U S1 140.91(2) 5 14_456 ?
S1 U S1 85.41(3) 14_556 14_456 ?
S1 U S1 73.53(3) 5_455 14_456 ?
S1 U S1 129.53(4) 5 14_456 ?
S2 U S1 71.270(15) 5_455 9_565 ?
S2 U S1 71.270(15) 5 9_565 ?
S1 U S1 136.504(16) 14_556 9_565 ?
S1 U S1 69.64(3) 5_455 9_565 ?
S1 U S1 69.64(3) 5 9_565 ?
S1 U S1 136.504(16) 14_456 9_565 ?
S2 U S1 71.270(15) 5_455 2_565 ?
S2 U S1 71.270(15) 5 2_565 ?
S1 U S1 69.64(3) 14_556 2_565 ?
S1 U S1 136.504(16) 5_455 2_565 ?
S1 U S1 136.504(16) 5 2_565 ?
S1 U S1 69.64(3) 14_456 2_565 ?
S1 U S1 127.45(4) 9_565 2_565 ?
S2 U Fe 125.164(15) 5_455 2_565 ?
S2 U Fe 125.164(15) 5 2_565 ?
S1 U Fe 45.381(16) 14_556 2_565 ?
S1 U Fe 91.46(2) 5_455 2_565 ?
S1 U Fe 91.46(2) 5 2_565 ?
S1 U Fe 45.381(16) 14_456 2_565 ?
S1 U Fe 153.72(2) 9_565 2_565 ?
S1 U Fe 78.83(2) 2_565 2_565 ?
S2 U Fe 125.164(15) 5_455 1_565 ?
S2 U Fe 125.164(15) 5 1_565 ?
S1 U Fe 91.46(2) 14_556 1_565 ?
S1 U Fe 45.381(16) 5_455 1_565 ?
S1 U Fe 45.381(16) 5 1_565 ?
S1 U Fe 91.46(2) 14_456 1_565 ?
S1 U Fe 78.83(2) 9_565 1_565 ?
S1 U Fe 153.72(2) 2_565 1_565 ?
Fe U Fe 74.888(5) 2_565 1_565 ?
S2 U U 46.50(2) 5_455 1_455 ?
S2 U U 133.50(2) 5 1_455 ?
S1 U U 132.705(14) 14_556 1_455 ?
S1 U U 47.294(14) 5_455 1_455 ?
S1 U U 132.705(14) 5 1_455 ?
S1 U U 47.294(14) 14_456 1_455 ?
S1 U U 90.0 9_565 1_455 ?
S1 U U 90.0 2_565 1_455 ?
Fe U U 90.0 2_565 1_455 ?
Fe U U 90.0 1_565 1_455 ?
S2 U U 133.50(2) 5_455 1_655 ?
S2 U U 46.50(2) 5 1_655 ?
S1 U U 47.294(14) 14_556 1_655 ?
S1 U U 132.705(14) 5_455 1_655 ?
S1 U U 47.294(14) 5 1_655 ?
S1 U U 132.705(14) 14_456 1_655 ?
S1 U U 90.0 9_565 1_655 ?
S1 U U 90.0 2_565 1_655 ?
Fe U U 90.0 2_565 1_655 ?
Fe U U 90.0 1_565 1_655 ?
U U U 180.0 1_455 1_655 ?
S2 U S2 136.50(2) 5_455 1_565 ?
S2 U S2 136.50(2) 5 1_565 ?
S1 U S2 64.77(2) 14_556 1_565 ?
S1 U S2 64.77(2) 5_455 1_565 ?
S1 U S2 64.77(2) 5 1_565 ?
S1 U S2 64.77(2) 14_456 1_565 ?
S1 U S2 116.27(2) 9_565 1_565 ?
S1 U S2 116.27(2) 2_565 1_565 ?
Fe U S2 37.444(2) 2_565 1_565 ?
Fe U S2 37.444(2) 1_565 1_565 ?
U U S2 90.0 1_455 1_565 ?
U U S2 90.0 1_655 1_565 ?
S2 U Fe 33.319(7) 5_455 5_455 ?
S2 U Fe 78.243(19) 5 5_455 ?
S1 U Fe 158.62(2) 14_556 5_455 ?
S1 U Fe 71.32(2) 5_455 5_455 ?
S1 U Fe 107.59(2) 5 5_455 ?
S1 U Fe 107.976(16) 14_456 5_455 ?
S1 U Fe 37.975(14) 9_565 5_455 ?
S1 U Fe 98.858(18) 2_565 5_455 ?
Fe U Fe 152.655(1) 2_565 5_455 ?
Fe U Fe 104.439(2) 1_565 5_455 ?
U U Fe 62.679(1) 1_455 5_455 ?
U U Fe 117.321(1) 1_655 5_455 ?
S2 U Fe 135.760(2) 1_565 5_455 ?
S2 U Fe 33.319(7) 5_455 6_455 ?
S2 U Fe 78.243(19) 5 6_455 ?
S1 U Fe 107.59(2) 14_556 6_455 ?
S1 U Fe 107.976(15) 5_455 6_455 ?
S1 U Fe 158.62(2) 5 6_455 ?
S1 U Fe 71.32(2) 14_456 6_455 ?
S1 U Fe 98.858(18) 9_565 6_455 ?
S1 U Fe 37.975(14) 2_565 6_455 ?
Fe U Fe 104.439(2) 2_565 6_455 ?
Fe U Fe 152.655(1) 1_565 6_455 ?
U U Fe 62.679(1) 1_455 6_455 ?
U U Fe 117.321(2) 1_655 6_455 ?
S2 U Fe 135.760(2) 1_565 6_455 ?
Fe U Fe 63.393(3) 5_455 6_455 ?
S2 U Fe 78.243(19) 5_455 5 ?
S2 U Fe 33.319(7) 5 5 ?
S1 U Fe 107.976(15) 14_556 5 ?
S1 U Fe 107.59(2) 5_455 5 ?
S1 U Fe 71.32(2) 5 5 ?
S1 U Fe 158.62(2) 14_456 5 ?
S1 U Fe 37.975(13) 9_565 5 ?
S1 U Fe 98.858(18) 2_565 5 ?
Fe U Fe 152.655(1) 2_565 5 ?
Fe U Fe 104.439(2) 1_565 5 ?
U U Fe 117.321(1) 1_455 5 ?
U U Fe 62.679(1) 1_655 5 ?
S2 U Fe 135.760(2) 1_565 5 ?
Fe U Fe 54.643(3) 5_455 5 ?
Fe U Fe 88.479(4) 6_455 5 ?
S2 Fe S2 180.0 9 . ?
S2 Fe S1 94.72(3) 9 13 ?
S2 Fe S1 85.28(3) . 13 ?
S2 Fe S1 85.28(3) 9 5_445 ?
S2 Fe S1 94.72(3) . 5_445 ?
S1 Fe S1 180.00(5) 13 5_445 ?
S2 Fe S1 94.72(3) 9 13_455 ?
S2 Fe S1 85.28(3) . 13_455 ?
S1 Fe S1 95.70(4) 13 13_455 ?
S1 Fe S1 84.30(4) 5_445 13_455 ?
S2 Fe S1 85.28(3) 9 5_545 ?
S2 Fe S1 94.72(3) . 5_545 ?
S1 Fe S1 84.30(4) 13 5_545 ?
S1 Fe S1 95.70(4) 5_445 5_545 ?
S1 Fe S1 180.00(5) 13_455 5_545 ?
S2 Fe U 76.45(3) 9 9_565 ?
S2 Fe U 103.55(3) . 9_565 ?
S1 Fe U 51.086(18) 13 9_565 ?
S1 Fe U 128.914(18) 5_445 9_565 ?
S1 Fe U 51.086(18) 13_455 9_565 ?
S1 Fe U 128.914(18) 5_545 9_565 ?
S2 Fe U 103.55(3) 9 1_545 ?
S2 Fe U 76.45(3) . 1_545 ?
S1 Fe U 128.914(18) 13 1_545 ?
S1 Fe U 51.086(18) 5_445 1_545 ?
S1 Fe U 128.914(18) 13_455 1_545 ?
S1 Fe U 51.086(18) 5_545 1_545 ?
U Fe U 180.000(4) 9_565 1_545 ?
S2 Fe Fe 90.0 9 1_655 ?
S2 Fe Fe 90.0 . 1_655 ?
S1 Fe Fe 42.149(18) 13 1_655 ?
S1 Fe Fe 137.851(18) 5_445 1_655 ?
S1 Fe Fe 137.851(18) 13_455 1_655 ?
S1 Fe Fe 42.149(18) 5_545 1_655 ?
U Fe Fe 90.0 9_565 1_655 ?
U Fe Fe 90.0 1_545 1_655 ?
S2 Fe Fe 90.0 9 1_455 ?
S2 Fe Fe 90.0 . 1_455 ?
S1 Fe Fe 137.851(18) 13 1_455 ?
S1 Fe Fe 42.149(18) 5_445 1_455 ?
S1 Fe Fe 42.149(18) 13_455 1_455 ?
S1 Fe Fe 137.851(18) 5_545 1_455 ?
U Fe Fe 90.0 9_565 1_455 ?
U Fe Fe 90.0 1_545 1_455 ?
Fe Fe Fe 180.0 1_655 1_455 ?
S2 Fe U 39.60(2) 9 13_455 ?
S2 Fe U 140.40(2) . 13_455 ?
S1 Fe U 134.29(2) 13 13_455 ?
S1 Fe U 45.71(2) 5_445 13_455 ?
S1 Fe U 91.01(2) 13_455 13_455 ?
S1 Fe U 88.99(2) 5_545 13_455 ?
U Fe U 104.439(2) 9_565 13_455 ?
U Fe U 75.561(2) 1_545 13_455 ?
Fe Fe U 117.321(1) 1_655 13_455 ?
Fe Fe U 62.679(1) 1_455 13_455 ?
S2 Fe U 140.40(2) 9 5_545 ?
S2 Fe U 39.60(2) . 5_545 ?
S1 Fe U 45.71(2) 13 5_545 ?
S1 Fe U 134.29(2) 5_445 5_545 ?
S1 Fe U 88.99(2) 13_455 5_545 ?
S1 Fe U 91.01(2) 5_545 5_545 ?
U Fe U 75.561(2) 9_565 5_545 ?
U Fe U 104.439(2) 1_545 5_545 ?
Fe Fe U 62.679(1) 1_655 5_545 ?
Fe Fe U 117.321(1) 1_455 5_545 ?
U Fe U 180.000(4) 13_455 5_545 ?
S2 Fe U 39.60(2) 9 13 ?
S2 Fe U 140.40(2) . 13 ?
S1 Fe U 91.01(2) 13 13 ?
S1 Fe U 88.99(2) 5_445 13 ?
S1 Fe U 134.29(2) 13_455 13 ?
S1 Fe U 45.71(2) 5_545 13 ?
U Fe U 104.439(2) 9_565 13 ?
U Fe U 75.561(2) 1_545 13 ?
Fe Fe U 62.679(1) 1_655 13 ?
Fe Fe U 117.321(2) 1_455 13 ?
U Fe U 54.643(3) 13_455 13 ?
U Fe U 125.357(3) 5_545 13 ?
S2 Fe U 140.40(2) 9 5_445 ?
S2 Fe U 39.60(2) . 5_445 ?
S1 Fe U 88.99(2) 13 5_445 ?
S1 Fe U 91.01(2) 5_445 5_445 ?
S1 Fe U 45.71(2) 13_455 5_445 ?
S1 Fe U 134.29(2) 5_545 5_445 ?
U Fe U 75.561(2) 9_565 5_445 ?
U Fe U 104.439(2) 1_545 5_445 ?
Fe Fe U 117.321(2) 1_655 5_445 ?
Fe Fe U 62.679(1) 1_455 5_445 ?
U Fe U 125.357(3) 13_455 5_445 ?
U Fe U 54.643(3) 5_545 5_445 ?
U Fe U 180.0 13 5_445 ?
S2 Fe S1 59.28(3) 9 9 ?
S2 Fe S1 120.72(3) . 9 ?
S1 Fe S1 127.92(2) 13 9 ?
S1 Fe S1 52.08(2) 5_445 9 ?
S1 Fe S1 127.92(2) 13_455 9 ?
S1 Fe S1 52.08(2) 5_545 9 ?
U Fe S1 135.726(13) 9_565 9 ?
U Fe S1 44.274(13) 1_545 9 ?
Fe Fe S1 90.0 1_655 9 ?
Fe Fe S1 90.0 1_455 9 ?
U Fe S1 39.301(9) 13_455 9 ?
U Fe S1 140.699(9) 5_545 9 ?
U Fe S1 39.301(9) 13 9 ?
U Fe S1 140.699(9) 5_445 9 ?
S2 Fe S1 120.72(3) 9 . ?
S2 Fe S1 59.28(3) . . ?
S1 Fe S1 52.08(2) 13 . ?
S1 Fe S1 127.92(2) 5_445 . ?
S1 Fe S1 52.08(2) 13_455 . ?
S1 Fe S1 127.92(2) 5_545 . ?
U Fe S1 44.275(13) 9_565 . ?
U Fe S1 135.725(13) 1_545 . ?
Fe Fe S1 90.0 1_655 . ?
Fe Fe S1 90.0 1_455 . ?
U Fe S1 140.699(9) 13_455 . ?
U Fe S1 39.301(9) 5_545 . ?
U Fe S1 140.699(9) 13 . ?
U Fe S1 39.301(9) 5_445 . ?
S1 Fe S1 180.0 9 . ?
Fe S1 Fe 95.70(4) 5 5_455 ?
Fe S1 U 83.533(9) 5 5_545 ?
Fe S1 U 153.26(4) 5_455 5_545 ?
Fe S1 U 153.26(4) 5 5_445 ?
Fe S1 U 83.533(9) 5_455 5_445 ?
U S1 U 85.41(3) 5_545 5_445 ?
Fe S1 U 96.31(2) 5 9_565 ?
Fe S1 U 96.31(2) 5_455 9_565 ?
U S1 U 110.36(3) 5_545 9_565 ?
U S1 U 110.36(3) 5_445 9_565 ?
Fe S1 Fe 127.92(2) 5 . ?
Fe S1 Fe 127.92(2) 5_455 . ?
U S1 Fe 69.38(2) 5_545 . ?
U S1 Fe 69.38(2) 5_445 . ?
U S1 Fe 56.895(18) 9_565 . ?
Fe S1 Fe 68.082(18) 5 6 ?
Fe S1 Fe 103.84(3) 5_455 6 ?
U S1 Fe 51.036(14) 5_545 6 ?
U S1 Fe 86.07(2) 5_445 6 ?
U S1 Fe 155.412(7) 9_565 6 ?
Fe S1 Fe 117.06(2) . 6 ?
Fe S1 Fe 103.84(3) 5 6_455 ?
Fe S1 Fe 68.082(18) 5_455 6_455 ?
U S1 Fe 86.07(2) 5_545 6_455 ?
U S1 Fe 51.036(14) 5_445 6_455 ?
U S1 Fe 155.412(7) 9_565 6_455 ?
Fe S1 Fe 117.06(2) . 6_455 ?
Fe S1 Fe 48.798(10) 6 6_455 ?
Fe S1 U 130.63(3) 5 9_465 ?
Fe S1 U 58.974(11) 5_455 9_465 ?
U S1 U 138.45(3) 5_545 9_465 ?
U S1 U 71.409(10) 5_445 9_465 ?
U S1 U 51.883(9) 9_565 9_465 ?
Fe S1 U 70.298(13) . 9_465 ?
Fe S1 U 152.411(14) 6 9_465 ?
Fe S1 U 103.668(5) 6_455 9_465 ?
Fe S1 U 58.974(11) 5 9_665 ?
Fe S1 U 130.63(3) 5_455 9_665 ?
U S1 U 71.409(10) 5_545 9_665 ?
U S1 U 138.45(3) 5_445 9_665 ?
U S1 U 51.883(9) 9_565 9_665 ?
Fe S1 U 70.298(13) . 9_665 ?
Fe S1 U 103.668(5) 6 9_665 ?
Fe S1 U 152.411(14) 6_455 9_665 ?
U S1 U 103.767(18) 9_465 9_665 ?
Fe S1 U 57.51(2) 5 . ?
Fe S1 U 57.51(2) 5_455 . ?
U S1 U 101.31(2) 5_545 . ?
U S1 U 101.31(2) 5_445 . ?
U S1 U 136.25(3) 9_565 . ?
Fe S1 U 166.85(2) . . ?
Fe S1 U 51.503(11) 6 . ?
Fe S1 U 51.503(11) 6_455 . ?
U S1 U 116.483(14) 9_465 . ?
U S1 U 116.483(14) 9_665 . ?
Fe S1 Fe 83.78(2) 5 6_454 ?
Fe S1 Fe 51.382(16) 5_455 6_454 ?
U S1 Fe 153.61(2) 5_545 6_454 ?
U S1 Fe 115.080(11) 5_445 6_454 ?
U S1 Fe 48.499(13) 9_565 6_454 ?
Fe S1 Fe 101.166(17) . 6_454 ?
Fe S1 Fe 141.20(2) 6 6_454 ?
Fe S1 Fe 119.464(14) 6_455 6_454 ?
U S1 Fe 46.942(7) 9_465 6_454 ?
U S1 Fe 82.224(14) 9_665 6_454 ?
U S1 Fe 91.152(16) . 6_454 ?
Fe S2 Fe 132.22(7) . 2 ?
Fe S2 U 107.085(17) . 5_545 ?
Fe S2 U 107.085(17) 2 5_545 ?
Fe S2 U 107.085(17) . 5_445 ?
Fe S2 U 107.085(17) 2 5_445 ?
U S2 U 87.00(4) 5_545 5_445 ?
Fe S2 U 66.11(3) . 1_545 ?
Fe S2 U 66.11(3) 2 1_545 ?
U S2 U 136.50(2) 5_545 1_545 ?
U S2 U 136.50(2) 5_445 1_545 ?
Fe S2 Fe 57.953(7) . 1_455 ?
Fe S2 Fe 110.89(2) 2 1_455 ?
U S2 Fe 137.68(3) 5_545 1_455 ?
U S2 Fe 64.688(3) 5_445 1_455 ?
U S2 Fe 77.590(19) 1_545 1_455 ?
Fe S2 Fe 110.89(2) . 2_655 ?
Fe S2 Fe 57.953(7) 2 2_655 ?
U S2 Fe 64.688(3) 5_545 2_655 ?
U S2 Fe 137.68(3) 5_445 2_655 ?
U S2 Fe 77.590(19) 1_545 2_655 ?
Fe S2 Fe 155.18(4) 1_455 2_655 ?
Fe S2 Fe 110.89(2) . 2_455 ?
Fe S2 Fe 57.953(7) 2 2_455 ?
U S2 Fe 137.68(3) 5_545 2_455 ?
U S2 Fe 64.688(3) 5_445 2_455 ?
U S2 Fe 77.590(19) 1_545 2_455 ?
Fe S2 Fe 58.045(5) 1_455 2_455 ?
Fe S2 Fe 115.905(13) 2_655 2_455 ?
Fe S2 Fe 57.953(7) . 1_655 ?
Fe S2 Fe 110.89(2) 2 1_655 ?
U S2 Fe 64.688(3) 5_545 1_655 ?
U S2 Fe 137.68(3) 5_445 1_655 ?
U S2 Fe 77.590(19) 1_545 1_655 ?
Fe S2 Fe 115.905(13) 1_455 1_655 ?
Fe S2 Fe 58.045(5) 2_655 1_655 ?
Fe S2 Fe 155.18(4) 2_455 1_655 ?
Fe S2 U 179.45(5) . 9_566 ?
Fe S2 U 47.230(17) 2 9_566 ?
U S2 U 73.300(18) 5_545 9_566 ?
U S2 U 73.300(18) 5_445 9_566 ?
U S2 U 113.337(17) 1_545 9_566 ?
Fe S2 U 122.046(6) 1_455 9_566 ?
Fe S2 U 68.880(3) 2_655 9_566 ?
Fe S2 U 68.880(3) 2_455 9_566 ?
Fe S2 U 122.046(6) 1_655 9_566 ?
Fe S2 U 47.230(17) . 9_565 ?
Fe S2 U 179.45(5) 2 9_565 ?
U S2 U 73.300(18) 5_545 9_565 ?
U S2 U 73.300(18) 5_445 9_565 ?
U S2 U 113.337(17) 1_545 9_565 ?
Fe S2 U 68.880(3) 1_455 9_565 ?
Fe S2 U 122.046(6) 2_655 9_565 ?
Fe S2 U 122.046(6) 2_455 9_565 ?
Fe S2 U 68.880(3) 1_655 9_565 ?
U S2 U 133.33(3) 9_566 9_565 ?
Fe S2 U 73.35(3) . 1_445 ?
Fe S2 U 73.35(3) 2 1_445 ?
U S2 U 178.53(3) 5_545 1_445 ?
U S2 U 91.529(11) 5_445 1_445 ?
U S2 U 44.972(12) 1_545 1_445 ?
Fe S2 U 41.315(8) 1_455 1_445 ?
Fe S2 U 116.55(3) 2_655 1_445 ?
Fe S2 U 41.315(8) 2_455 1_445 ?
Fe S2 U 116.55(3) 1_655 1_445 ?
U S2 U 106.276(8) 9_566 1_445 ?
U S2 U 106.275(8) 9_565 1_445 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U S2 2.7609(11) 5_455 ?
U S2 2.7609(11) 5 ?
U S1 2.8021(7) 14_556 ?
U S1 2.8021(7) 5_455 ?
U S1 2.8021(7) 5 ?
U S1 2.8021(7) 14_456 ?
U S1 2.9820(10) 9_565 ?
U S1 2.9820(10) 2_565 ?
U Fe 3.57828(18) 2_565 ?
U Fe 3.57828(18) 1_565 ?
U U 3.8009 1_455 ?
U U 3.8009 1_655 ?
U S2 3.8046(15) 1_565 ?
U Fe 4.14059(17) 5_455 ?
U Fe 4.14059(17) 6_455 ?
U Fe 4.14059(17) 5 ?
Fe S2 2.3794(6) 9 ?
Fe S2 2.3794(6) . ?
Fe S1 2.5633(7) 13 ?
Fe S1 2.5633(7) 5_445 ?
Fe S1 2.5633(7) 13_455 ?
Fe S1 2.5633(7) 5_545 ?
Fe U 3.57828(18) 9_565 ?
Fe U 3.57828(18) 1_545 ?
Fe Fe 3.8009 1_655 ?
Fe Fe 3.8009 1_455 ?
Fe U 4.14059(16) 13_455 ?
Fe U 4.14059(16) 5_545 ?
Fe U 4.14059(16) 13 ?
Fe U 4.14059(16) 5_445 ?
Fe S1 4.1908(11) 9 ?
Fe S1 4.1908(11) . ?
S1 Fe 2.5633(7) 5 ?
S1 Fe 2.5633(7) 5_455 ?
S1 U 2.8021(7) 5_545 ?
S1 U 2.8021(7) 5_445 ?
S1 U 2.9821(10) 9_565 ?
S1 Fe 4.6006(9) 6 ?
S1 Fe 4.6006(9) 6_455 ?
S1 U 4.8311(6) 9_465 ?
S1 U 4.8311(6) 9_665 ?
S1 Fe 5.4626(9) 6_454 ?
S2 Fe 2.3794(6) 2 ?
S2 U 2.7609(11) 5_545 ?
S2 U 2.7609(11) 5_445 ?
S2 U 3.8047(15) 1_545 ?
S2 Fe 4.4843(3) 1_455 ?
S2 Fe 4.4843(3) 2_655 ?
S2 Fe 4.4843(3) 2_455 ?
S2 Fe 4.4843(3) 1_655 ?
S2 U 4.7388(6) 9_566 ?
S2 U 4.7388(6) 9_565 ?
S2 U 5.3780(11) 1_445 ?
